Chapter 5: Diffusion. 5.1 SteadyState Diffusion


 Ashlee Carpenter
 1 years ago
 Views:
Transcription
1 : Diffusion Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Diffusion is process which is NOT due to the action of a force, but a result of the random movements of atoms (statistical problem) 1. Diffusivity and Fick s laws. Atomistic mechanisms of diffusion 3. Temperature dependence and Arrenius plot 4. Industrial applications  carburized steel,  dopants in silicon 5.1 SteadyState Diffusion Consider diffusion of solute atoms (b) in solid state solution (AB) in direction between two parallel atomic planes (separated by ) if there is no changes with time in C B at these planes such diffusion condition is called steadystate diffusion For a steadystate diffusion, flu (flow), J, of atoms is: dc J = D d J flu of atoms, atoms/(m s): the number of particles which pass through a unit area in a unit of time; D diffusivity or diffusion coefficient, m /s dc/d concentration gradient, atoms/m 4 Recall: Solvent the majority atom type (or host atoms): Solute the element with lower concentration Substitutional a solid solution in which the solute atoms are replaced by solute Interstitial solute atoms are located in gaps between host atoms 1
2 Fick s first law of diffusion dc J = D d atoms m J = D m s s  sign: flu direction is from the higher to the lower concentration; i.e. it is the opposite to the concentration gradient For steadystate diffusion condition (no change in the system with time), the net flow of atoms is equal to the diffusivity D times the diffusion gradient dc/d dc atoms 1 3 d m m Diffusivity D depends on: 1. Diffusion mechanism. Temperature of diffusion 3. Type of crystal structure (bcc > fcc) 4. Crystal imperfections 5. Concentration of diffusing species NonSteadyState Diffusion In practice the concentration of solute atoms at any point in the material changes with time nonsteadystate diffusion For nonsteadystate condition, diffusion coefficient, D  NOT dependent on time: Second Fick s law of diffusion: If D D(), in 1D case: dc dt = dc dt d d dc D d C = D Change in concentration in semiinfinite rods of Cu and Ni caused by diffusion, From G. Gottstein Physical Foundations of Material Science The rate of compositional change is equal to the diffusivity times the rate of the change of the concentration gradient In 3D case: dc dt C C C D + + y z =
3 NonSteadyState Diffusion (continued) With specific initial or boundary conditions this partial differential equations can be solved to give the concentration as function of spatial position and time c(, y, z, t) Let us consider two rods with different concentrations c 1 and c which are joined at =0 and both are so long that mathematically they can be considered as infinitely long The concentration profile at t = 0 is discontinuous at = 0: < 0, c = c 1 ; < 0, c = c dc We can obtain solution of: C = D dt c c(, t) c = where erf ( z) = z = Dt 1 c π 1 π z 0 Dt e e ξ ξ c dξ = c erf Dt dξ, is known as the error function Gas diffusion into a solid Let us consider the case of a gas A diffusing into a solid B Gas A Solid B Cs C C C S o = erf Dt = 0 C S surf. C of element in gas diffusing into the surface C o initial uniform concentration of element in solid  distance from surface D diffusivity of diffusing solute element t time erf mathematical function called error function 3
4 Error function Curve of the error function erf (z) for z = Dt Q: Consider the gas carburizing of a gear of 1018 steel (C 0.18 wt %) at 97 C. Calculate the time necessary to increase the C content to 0.35 wt % at 0.40 mm below the surface of the gear. Assume the C content at the surface to be 1.15 wt % and that the nominal C content of the steel gear before carburizing is 0.18 wt %. D (C in γ iron) at 97 C = m /s 4
5 5. Atomistics of Solid State Diffusion Diffusion mechanisms: 1. Vacancy (substitutional) diffusion migration of atom in a lattice assisted by the presence of vacancies E.: self diffusion of Cu atoms in Cu crystal. Interstitial diffusion movement of atoms from one interstitial site to another neighboring interstitial site without permanent displacement any of the atoms in the matri crystal lattice E.: C diffusion in BCC iron Vacancies The simplest point defect is the vacancy (V) an atom site from which an atom is missing Vacancies are always present; their number N V depends on temperature (T) N V = N e EV kt N V  # of vacancies N  number of lattice sites E V energy required to form a vacancy k Boltzmann constant k = J K 1 ; or ev K 1 T absolute temperature vacancy 5
6 Vacancy (Substitutional) Diffusion Mechanism Substitutional (in homogeneous system  selfdiffusion, in heterogeneous system solid state solutions) Vacancies are always present at any T As T increases # of vacancies increases diffusion rate increases Move atom A (from (1) to ()) = move vacancy from () to (1)..? higher T melt stronger bonding between atoms high activation energy to move V Kirkendall effect Marker at the diffusion interface move slightly in the opposite direction to the most rapidly moving species vacancies can move! 6
7 Possible mechanisms of selfdiffusion and their activation energy 1. Neighboring atoms echange sites. Ring mechanism 3. Vacancy mechanism 4. Direct interstitial mechanism 5. Indirect interstitial mechanism Migration Formation Total ev 1 ev  1 ev 8 ev ev ev 3.4 ev 4 ev 6 0. ev 3.4 ev 3.6 ev Anisotropy Effects From G.Gottstein Physical Foundations of Material Science 7
8 Carbon diffusion in Fe Jump frequency Γ [s 1 ] of an atom is given by: Γ = ν kt e G m Usually ν [s 1 ] vibrational frequency of the atom There is a fundamental relationship between the jump frequency Γ and the diffusion coefficient D which is independent of mechanism and crystal structure: λ λ D = Γ = 6 6τ λ the jump distance of the diffusing atom τ =1/Γ the time interval between two jumps J = J MN  J NM A 1 J = C M Γ C 4 3 D = Γa 4 A N 1 Γ 4 3 Carbon diffusion in Fe Can be derived from an atomistic considerations of the diffusion processes C atoms are located on the octahedral interstitial sites (black circles) J = J MN  J NM Only ¼ of possible jumps of C atoms lead to flu in + Only /3 of all C atoms can jump in direction λ λ D = Γ = 6 6τ D = Γa 4 8
9 5.3 Effects of T on diffusion in solids Diffusion rate in a system will increase with temperature: D = D e o EA RT D diffusivity, m /s D 0 proportionality constant, m /s, independent of T E A activation energy for diffusing species, J/mol R molar gas constant R = J mol1 K1; or 1.987cal mol1k1 T absolute temperature Activation energy A + B C + D A (initial state) A* (final state) only a fraction of the molecules or atoms in a system will have sufficient energy to reach E* A thermally active process is one which requires a definite amount of thermal energy to overcome an activation energy barrier and enter the reactive state 9
10 Bolzmann s equation On the basis of statistical analysis, Bolzmann s results showed that the probability of finding a molecule or atom at an energy level E * > the average energy E of all the molecules or atoms in a system at a particular temperature T, K, was: Probability e * E E kt where k B = J/(atom K)  Boltzmann s constant The fraction of atoms or molecules in a system having energies > E* at a given T (where E* is much greater than the average energy of any atom or molecule: n N total = C e * E kt Arrhenius Rate Equation The rate of many chemical reaction as a function of temperature as follows: Rate _ of _ reaction = C e E A RT C rate constant, independent of T E A activation energy R molar gas constant R = J mol 1 K 1 ; or 1.987cal mol 1 K 1 T absolute temperature 10
11 If we rewrite in natural log plot: EA ln rate = ln C RT ln rate = a ln C = b y = b + m 1 = T Typical Arrhenius Plot or in logarithmic log plot: log rate = log10 C 10 EA.303RT Q.: The diffusivity of Ag atoms in solid silver metal is 1.0X10 17 m /s at 500 o C and m /s at 1000 o C. Calculate the activation energy (J/mole) for the diffusion of Ag in Ag in the T range 500 to 1000 o C. 11
12 5.4 Industrial applications Steel Hardening by Gas Carburizing In the gas carburizing process for steel parts, the parts are placed in a furnace in contact with a gas rich in COCH 4 miture at ~97ºC. Fe + CH 4 FeC ( = % C), T = 97 o C The C from the gas diffuses into the surface of the steel part and increases the C content of the outer surface region of the part. The higher C concentration at the surface makes the steel harder in this region A steel part can thus be produced with a hard outer layer and a tough low C steel inner core (important, for eample, for many types of gears) Dopants activation Dopants can be incorporated into Si wafer to change their electrical conducting characteristics mask B, P + Ion implantation Annealing 1
13 Q: If boron, B, is diffused into a thick slice of Si with no previous B in it at a temperature of 1100 C for 5 h, what is the depth below the surface at which the concentration is atoms/cm 3 if the surface concentration is atoms/cm3? D = cm /s for B diffusing in Si at 1100 C. Summary Diffusion: the movement of particles in a solid from an area of high concentration to an area of low concentration, resulting in the uniform distribution of the substance Fick s first diffusion law: for steadystate diffusion condition (no change in the system with time), the net flow of atoms is equal to the diffusivity D times the diffusion gradient dc/d J = D Fick s second diffusion law: The rate of compositional change is equal to the diffusivity times the rate of the change of the concentration gradient Diffusion rate in a system will increase with temperature: D = D e o dc d dc C = D dt EA RT 13
Materials Science and Engineering I. Chapter 5
Materials Science and Engineering I Chapter 5 Outline of Chapter 5 Rate processes in Solids Atomic diffusion in solids Diffusion mechanisms Vacancy or Substitutional Diffusion Mechanism Interstitial
More informationChapter Outline. Diffusion  how do atoms move through solids?
Chapter Outline iffusion  how do atoms move through solids? iffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities The mathematics of diffusion Steadystate diffusion (Fick s first law)
More informationTHE WAY TO SOMEWHERE. Subtopics. Diffusion Diffusion processes in industry
THE WAY TO SOMEWHERE Subtopics 1 Diffusion Diffusion processes in industry RATE PROCESSES IN SOLIDS At any temperature different from absolute zero all atoms, irrespective of their state of aggregation
More informationChapter 5: Diffusion in Solids. Diffusion
/8/0 Chapter 5: Diffusion in Solids ISSUES TO ADDRESS... How does diffusion occur? Why is it an important part of processing? How can the rate of diffusion be predicted for some simple cases? How does
More informationIntroduction To Materials Science FOR ENGINEERS, Ch. 5. Diffusion. MSE 201 Callister Chapter 5
Diffusion MSE 21 Callister Chapter 5 1 Goals: Diffusion  how do atoms move through solids? Fundamental concepts and language Diffusion mechanisms Vacancy diffusion Interstitial diffusion Impurities Diffusion
More informationFoundations of Materials Science and Engineering Lecture Note 8 (Chapter 5 Diffusion)
Foundations of Materials Science and Engineering Lecture Note 8 (Chapter 5 Diffusion) May 13, 2013 Kwang Kim Yonsei University kbkim@yonsei.ac.kr 39 8 7 34 53 Y O N Se I 88.91 16.00 14.01 78.96 126.9 Introduction
More informationDiffusion. Diffusion in Materials Q. How do changes in microstructure and chemical. Atomic Motion in Solids
Diffusion Atomic Motion in Solids Week6 Material Sciences and Engineering MatE271 1 Diffusion in Materials Q. How do changes in microstructure and chemical composition actually occur? A. Atoms must be
More informationVACANCY DIFFUSION. substitutional impurity atom
CASE HARDENING This steel gear has been case hardened  a process in which carbon atoms have been diffused into the surface of the steel. This increases the surficial carbon content of the steel, making
More information! The mathematics of diffusion
Chapter Outline Diffusion  how do atoms move through solids?! Diffusion mechanisms " Vacancy diffusion " Interstitial diffusion " Impurities! The mathematics of diffusion " Steadystate diffusion (Fick
More informationIn order to solve this problem it is first necessary to use Equation 5.5: x 2 Dt. = 1 erf. = 1.30, and x = 2 mm = 2 103 m. Thus,
5.3 (a) Compare interstitial and vacancy atomic mechanisms for diffusion. (b) Cite two reasons why interstitial diffusion is normally more rapid than vacancy diffusion. Solution (a) With vacancy diffusion,
More informationMAE 20 Winter 2011 Assignment 3 solutions
MAE 20 Winter 2011 Assignment 3 solutions 4.3 Calculate the activation energy for vacancy formation in aluminum, given that the equilibrium number of vacancies at 500 C (773 K) is 7.57 10 23 m 3. The
More informationThe photograph at the top of this page is of a steel gear that has
Chapter 5 Diffusion The photograph at the top of this page is of a steel gear that has been case hardened. Its outer surface layer was selectively hardened by a hightemperature heat treatment during which
More informationLecture 3: Introduction to Diffusion
Materials Science & Metallurgy Master of Philosophy, Materials Modelling, Course MP6, Kinetics and Microstructure Modelling, H. K. D. H. Bhadeshia Lecture 3: Introduction to Diffusion Mass transport in
More information14:635:407:02 Homework III Solutions
14:635:407:0 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 37 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationMaterials Science and Engineering Department MSE , Sample Test #1, Spring 2010
Materials Science and Engineering Department MSE 200001, Sample Test #1, Spring 2010 ID number First letter of your last name: Name: No notes, books, or information stored in calculator memories may be
More informationImpurity Diffusion. Fundamental process step for microelectronics. We want Substitutional diffusion
Diffusion Impurity Diffusion Fundamental process step for microelectronics Controls majority carrier type Controls semiconductor resistivity We want Substitutional diffusion Needed to provide carriers
More informationDIFFUSION IN SOLIDS. Materials often heat treated to improve properties. Atomic diffusion occurs during heat treatment
DIFFUSION IN SOLIDS WHY STUDY DIFFUSION? Materials often heat treated to improve properties Atomic diffusion occurs during heat treatment Depending on situation higher or lower diffusion rates desired
More informationCHAPTER 6 DIFFUSION PROBLEM SOLUTIONS. 6.1 Briefly explain the difference between selfdiffusion and interdiffusion.
CHAPTER 6 DIFFUSION PROBLEM SOLUTIONS Introduction 6.1 Briefly explain the difference between selfdiffusion and interdiffusion. Selfdiffusion is atomic migration in pure metals i.e., when all atoms exchanging
More information14:635:407:02 Homework III Solutions
14:635:407:02 Homework III Solutions 4.1 Calculate the fraction of atom sites that are vacant for lead at its melting temperature of 327 C (600 K). Assume an energy for vacancy formation of 0.55 ev/atom.
More informationToday s Topics... Lecture 7. A.K.M.B. Rashid Department of MME, BUET
Lecture 7 Diffusion Ref: 1. WD Callister Jr. Materials Science and Engineering: An Introduction, John Wiley & Sons. 2. DA Askeland. The Science and Engineering of Materials, Chapman & Hall. A.K.M.B. Rashid
More informationDiffusion. J =  D dc dx { =  D C in 3dimensions} [J] = #/cm 2 s [C] = #/cc [D] = cm 2 /s note  J along negative concentration gradient
Diffusion Diffusion is the relative movement of atoms in a solid, liquid or gas concerned here with diffusion in solids. Is very important in 1. phase transformations. corrosion resistant coatings 3. separation
More informationCh. 4: Imperfections in Solids Part 1. Dr. Feras Fraige
Ch. 4: Imperfections in Solids Part 1 Dr. Feras Fraige Outline Defects in Solids 0D, Point defects vacancies Interstitials impurities, weight and atomic composition 1D, Dislocations edge screw 2D, Grain
More informationCHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS
41 CHAPTER 4 IMPERFECTIONS IN SOLIDS PROBLEM SOLUTIONS Vacancies and SelfInterstitials 4.1 In order to compute the fraction of atom sites that are vacant in copper at 1357 K, we must employ Equation
More informationModule 4. Atomic mechanism of diffusion. Till now, we discussed the diffusion process without going to the atomic level.
Module 4 Atomic mechanism of diffusion Till now, we discussed the diffusion process without going to the atomic level. By measuring concentration profile, one can measure the diffusion coefficients. However,
More informationImperfections in atomic arrangements
MME131: Lecture 8 Imperfections in atomic arrangements Part 1: 0D Defects A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Occurrence and importance of crystal defects Classification
More informationDefects Introduction. Bonding + Structure + Defects. Properties
Defects Introduction Bonding + Structure + Defects Properties The processing determines the defects Composition Bonding type Structure of Crystalline Processing factors Defects Microstructure Types of
More informationSection 4: Thermal Oxidation. Jaeger Chapter 3. EE143  Ali Javey
Section 4: Thermal Oxidation Jaeger Chapter 3 Properties of O Thermal O is amorphous. Weight Density =.0 gm/cm 3 Molecular Density =.3E molecules/cm 3 O Crystalline O [Quartz] =.65 gm/cm 3 (1) Excellent
More informationOxidation of silicon is an important process in VLSI. The typical roles of SiO 2 are: 1. mask against implant or diffusion of dopant into silicon
Chapter 4 1 CHAPTER 4: Oxidation Oxidation of silicon is an important process in VLSI. The typical roles of SiO 2 are: 1. mask against implant or diffusion of dopant into silicon 2. surface passivation
More informationLecture'5' Diffusion'
Lecture'5' Diffusion' Aaron'D.'Franklin' CHEM%548,%Duke%University% Solid&State/MaterialChemistry Slide%1% Diffusion% Diffusion  Mass transport by atomic motion Mechanisms Gases & Liquids random (Brownian)
More informationSurface Treatments. Corrosion Protective coatings for harsh environments (catalytic converters, electrochemical cells )
Surface Treatments Applications Biomedical (biocompatible coatings on implants, drug coatings for sustained release ) Mechanical Tribological friction and wear (tool steels, implants ) Fatigue minimize
More informationSolution: ΔG = a 3 ΔG v. + 6a 2 γ. Differentiation of this expression with respect to a is as. d ΔG da = d(a3 ΔG v. + d(6a2 γ) = 3a 2 ΔG v.
14:440:407 ch10 Question 10.2: (a) Rewrite the expression for the total free energy change for nucleation (Equation 10.1) for the case of a cubic nucleus of edge length a (instead of a sphere of radius
More informationDefects in Solids Imperfections in Solids : Examples of the large impact of defects Gemstones Metals Defect Classification:
Defects in Solids Imperfections in Solids : Materials are often stronger when they have defects. The mechanical and electrical properties of a material are affected by the presence of defects. The study
More informationISSUES TO ADDRESS... Transforming one phase into another takes time.
ISSUES TO ADDRESS... Transforming one phase into another takes time. Fe C FCC Fe g 3 C Eutectoid transformation (cementite) (Austenite) + a (ferrite) (BCC) How does the rate of transformation depend on
More informationCHAPTER 3 OUTLINE. DIFFUSION and IMPERFECTIONS IN SOLIDS
CHAPTER 3 DIFFUSION and IMPERFECTIONS IN SOLIDS OUTLINE 1. TYPES OF DIFFUSIONS 1.1. Interdiffusion 1.2. Selfdiffusion 1.3.Diffusion mechanisms 1.4.Examples 2. TYPES OF IMPERFECTIONS 2.1.Point Defects 2.2.Line
More informationChapter Understand the factors that affect metal solubility and be able to give rough predictions of when metals are mutually soluble.
hapter 5 Highlights:. Be able to recognize and discriminate between different point and extended defects in metals and ceramics. Know the direction of the Burger's vector for extended defects.. Given the
More information in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons
Free Electrons in a Metal  in a typical metal each atom contributes one electron to the delocalized electron gas describing the conduction electrons  if these electrons would behave like an ideal gas
More informationChapter Outline Microscopy 4.11 Grain size determination
Crystals are like people, it is the defects in them which tend to make them interesting!  Colin Humphreys. Defects in Solids 0D, Point defects vacancies interstitials impurities, weight and atomic composition
More informationThe University of Western Ontario Department of Physics and Astronomy P2800 Fall 2008
P2800 Fall 2008 Questions (Total  20 points): 1. Of the noble gases Ne, Ar, Kr and Xe, which should be the most chemically reactive and why? (0.5 point) Xenon should be most reactive since its outermost
More informationVysoká škola báňská Technická univerzita Ostrava. Physical Metallurgy. Didactic Text. Jaroslav Sojka
Vysoká škola báňská Technická univerzita Ostrava Physical Metallurgy Didactic Text Jaroslav Sojka Ostrava 2013 Physical Metallurgy Review: Prof. Ing. Ludmila Hypecká, DrSc. Description: Physical Metallurgy
More informationThe atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C. = 2(sphere volume) = 2 = V C = 4R
3.5 Show that the atomic packing factor for BCC is 0.68. The atomic packing factor is defined as the ratio of sphere volume to the total unit cell volume, or APF = V S V C Since there are two spheres associated
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS
CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS ISSUES TO ADDRESS... PLASTIC DEFORMATION and DISLOCATIONS * Dislocation motion * Slip in: single crystals polycrystalline materials * Dislocation motion
More informationCHAPTER 6: DIFFUSION IN SOLIDS. Interdiffusion. Simple Diffusion. Diffusion Steady and NonSteady State ISSUES TO ADDRESS...
CHAPTER 6: DIFFUSION IN SOLIDS Diffusion Steady and NonSteady State ISSUES TO ADDRESS... Gear from casehardened steel (C diffusion) Diffusion  Mass transport by atomic motion How does diffusion occur?
More informationLecture 5: Diffusion Coefficient (Diffusivity)
Lecture 5: Diffusion Coefficient (Diffusivity) Today s topics Understand the general physical meaning of diffusion coefficient. What is chemical diffusion coefficient (D C ) and tracer diffusion coefficient
More informationCHAPTER 8: Diffusion. Chapter 8
1 CHAPTER 8: Diffusion Diffusion and ion implantation are the two key processes to introduce a controlled amount of dopants into semiconductors and to alter the conductivity type. Figure 8.1 compares these
More informationLecture 4 Dislocations & strengthening mechanisms
Lecture 4 Dislocations & strengthening mechanisms ISSUES TO ADDRESS... Why are dislocations observed primarily in metals and alloys? How are strength and dislocation motion related? How do we increase
More informationCHAPTER 4: IMPERFECTIONS IN SOLIDS
CHAPTER 4: IMPERFECTIONS IN SOLIDS ISSUES TO ADDRESS... What types of defects arise in solids? Can the number and type of defects be varied and controlled? How do defects affect material properties? Are
More informationDr. M. Medraj Mech. Eng. Dept.  Concordia University MECH 221 lecture 21/2
ELECTRICAL PROPERTIES OUTLINE INTRODUCTION ELECTRICAL CONDUCTION ENERGY BAND STRUCTURE IN SOLIDS INSULATORS AND SEMICONDUCTORS METALS: ELECTRON MOBILITY INFLUENCE OF TEMPERATURE INFLUENCE OF IMPURITY SEMICONDUCTORS
More informationElectrical Properties
Chapter 12 Electrical Properties QUESTIONS AND PROBLEMS Ohm s Law Electrical Conductivity W12.1 An aluminum wire 10 m long must experience a voltage drop of less than 1.0 V when a current of 5 A passes
More informationMechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied
Mechanical Properties of Metals Mechanical Properties refers to the behavior of material when external forces are applied Stress and strain fracture or engineering point of view: allows to predict the
More informationOverview of Silicon Device Physics
Overview of Silicon Device Physics Dr. David W. Graham West Virginia University Lane Department of Computer Science and Electrical Engineering 1 Silicon Si has 14 Electrons Silicon is the primary semiconductor
More informationLecture 24: Doping. 1 Introduction 1. 2 Thermal diffusion Diffusion sources Drivein... 6
Lecture 24: Doping Contents 1 Introduction 1 2 Thermal diffusion 2 2.1 Diffusion sources......................... 5 2.2 Drivein.............................. 6 3 Diffusion concentration gradients 7 3.1
More informationSteadystate diffusion experiments
DIFFUSION IN SOLIDS Steadystate diffusion experiments (13.1) (13.2) r 1, r 2 : inside and outside radii of the tube C1, C2: corresponding concentrations of carbon at these surfaces For steady state,
More informationLecture 4: Silicon Oxidation
Lecture 4: Silicon Oxidation Topics covered: Thermal Oxidation process to form SiO 2. Impurity redistribution during oxidation. Material properties and thickness measurement techniques for SiO 2. MOSFET
More informationThermodynamics and Kinetics
Thermodynamics and Kinetics A Little Justification Thin film growth is intimately intertwined with thermodynamics and gas kinetics. Temperature and pressure are the main parameters of film growth, especially
More informationImperfections in Solids
Chapter 5 Imperfections in Solids QUESTIONS AND PROBLEMS Point Defects in Metals W5.1 Calculate the number of vacancies per cubic meter in gold at 900 C. The energy for vacancy formation is 0.98 ev/atom.
More informationMaterials and Devices in Electrical Engineering
Examination Materials and Devices in Electrical Engineering Monday 19 th of March, 14:00 to 16:00, room 108 FZU/AVG It is allowed to use any kind of media (books, scripts, overheads, notes,...) during
More informationDOPING BY DIFFUSION AND IMPLANTATION
DOPING BY DIFFUSION AND IMPLANTATION 7 th IndoGerman Winter Academy2008 Presented by Niranjan Patil IIT Bombay, Course 3 Tutor: Prof N. Dasgupta IIT Madras Doping by Diffusion & Implantation 1 Outline
More informationOptoelectronic Materials and Devices Prof. Dr. Monica Katiyar Department of Materials Science and Engineering Indian Institute of Technology, Kanpur
Optoelectronic Materials and Devices Prof. Dr. Monica Katiyar Department of Materials Science and Engineering Indian Institute of Technology, Kanpur Module  3 Optoelectronic Device Physics Lecture  21
More informationElectrical properties
Electrical properties ELECTRICAL CONDUCTION ENERGY BAND STRUCTURE IN SOLIDS INSULATORS AND SEMICONDUCTORS METALS: ELECTRON MOBILITY INFLUENCE OF TEMPERATURE INFLUENCE OF IMPURITY SEMICONDUCTORS PN RECTIFYING
More informationChapter 3: Kinetics of Electrode Reactions
Goal: To understand the observed behavior of electrode kinetics with respect to potential and concentration. = i/nfa (mol/scm 2 ) Rate = f(e) Dynamic Equilibrium A k f k b B s 1 f = k f C A (M/s) b =
More informationMATERIALS SCIENCE. PHASE DIAGRAMS 1) Introduction
MATEIALS SCIENCE 1) Introduction A phase diagram is a plot showing the phases of a substance at various temperatures and pressures. Usually pressure vs. temperature or temperature vs. composition graph
More informationDISLOCATIONS AND STRENGTHENING MECHANISMS. IE114 Materials Science and General Chemistry Lecture7
DISLOCATIONS AND STRENGTHENING MECHANISMS IE114 Materials Science and General Chemistry Lecture7 StressStrain Curves Typical StressStrain Curve of NonFerrous Alloys (Al, Cu, etc..) Yield point ( y
More informationThe Iron Iron Carbide (Fe Fe 3 C) Phase Diagram
The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram Reactions Peritectic L + δ = γ at T=1493 o C and 0.18wt%C Eutectic L = γ + Fe 3 C at T=1147 o C and 4.3wt%C Eutectoid γ = α + Fe 3 C at T=727 o C and 0.77wt%C
More informationDoping and Silicon Reference: Chapter 4 Jaeger or Chapter 3 Ruska Recall dopants in silicon (column IV element) Column V extra electrons N type
Doping and Silicon Reference: Chapter 4 Jaeger or Chapter 3 Ruska Recall dopants in silicon (column IV element) Column V extra electrons N type dopant N D P Phospherus, As Arsenic & Sb Antimony most common
More informationCHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS
71 CHAPTER 7 DISLOCATIONS AND STRENGTHENING MECHANISMS PROBLEM SOLUTIONS Basic Concepts of Dislocations Characteristics of Dislocations 7.1 The dislocation density is just the total dislocation length
More informationPLAYING WITH PROPERTIES. Subtopics. Strengthening mechanisms Heat treatment Hot working
PLAYING WITH PROPERTIES Subtopics 1 Strengthening mechanisms Heat treatment Hot working CAN SLIP PROCESS BE CONTROLLED? If the dislocation at point A moves to the left, it is blocked by the point defect.
More informationWhy are defects important? Chapter Outline. Bonding + Crystal Structure + Properties. Defects Microscopy 4.11 Grain size determination
rystals are like people, it is the defects in them which tend to make them interesting!  olin Humphreys. Defects in Solids hapter Outline 0D, Point defects vacancies interstitials impurities, weight and
More informationOverview. Metals. Metals. Metallic Bonding. Metallic Structure. Metallic Bonding. Atomic structure  metallic bond, lattice, unit cell, allotropy
Overview Metals Dr. Kimberly Kurtis School of Civil Engineering Georgia Institute of Technology Atlanta, Georgia Atomic structure  metallic bond, lattice, unit cell, allotropy Microstructure  grains,
More informationChapter Outline. Defects Introduction (I)
Crystals are like people, it is the defects in them which tend to make them interesting!  Colin Humphreys. Defects in Solids Chapter Outline 0D, Point defects vacancies interstitials impurities, weight
More informationSOLID STATE 17. Packing and Defects. 1. Point Defects Vacancies, Interstitials and Frenkel Defects
SOLID STATE 17 Packing and Defects 1. Point Defects Vacancies, Interstitials and Frenkel Defects For a crystal containing N atoms, there is an equilibrium number of vacancies, n v, at a temperature T (in
More informationAdvanced Inorganic Chemistry (CHE 510) Final Examination December 16, 2005
Advanced Inorganic Chemistry (CHE 510) Final Examination December 16, 2005 Name: Answer questions in the area provided, the back of an exam page, or on the clearly labeled spare sheet. Please show all
More informationChapter Outline: Phase Transformations in Metals
Chapter Outline: Phase Transformations in Metals Heat Treatment (time and temperature) Microstructure Mechanical Properties Kinetics of phase transformations Multiphase Transformations Phase transformations
More informationPhase diagrams assist in the interpretation of microstructure of metals.
Phase equilibrium diagrams. Overview Phase diagrams assist in the interpretation of microstructure of metals. Traditional sectioning, mounting, polishing and etching techniques are often used to determine
More informationApplications of solid ionic conductors. Membranes in separation processes Electrolytes in sensors Electrolytes in fuel cells and batteries
Ionic conductors Ionic solids contain defects that allow the migration of ions in an electric field Some solid materials have very high ionic conductivities at reasonable temperatures useful in solid state
More information4.2.4 Chemical Diffusion Coefficient
4.2. CHEMICAL DRIVING FORCE 107 we see that the first term in this expression comes from the concentration driving force arising from the ideal entropy of mixing, and the second term arises from the nonideality
More informationChapter Outline Dislocations and Strengthening Mechanisms
Chapter Outline Dislocations and Strengthening Mechanisms What is happening in material during plastic deformation? Dislocations and Plastic Deformation Motion of dislocations in response to stress Slip
More informationSOLIDIFICATION. METE 327, Fall METE 327 Physical Metallurgy Copyright 2008 Loren A. Jacobson 5/16/08
SOLIDIFICATION METE 327, Fall 2008 OUTLINE The Liquid Phase Nucleation Crystal Growth, SolidLiquid Interface Dendritic Growth Freezing in Alloys Freezing of Ingots Eutectic Freezing Metallic Glass SOLIDIFICATION
More informationImperfections, Defects and Diffusion
Imperfections, Defects and Diffusion Lattice Defects Week5 Material Sciences and Engineering MatE271 1 Types of Defects o Point defects (composition) Vacancies Interstitials (missing atoms) (extra atoms)
More informationElectrons in atoms and solids. Review: Pauli Exclusion Principle. Stimulated Emission. Bosons and fermions. Problem (continued)
lectrons in atoms and solids TODAY: Lasers and population inversion nergy bands in solids The Boltzmann factor Thermal distribution of electrons Review: Pauli xclusion Principle No two electrons in the
More informationECE 340 Lecture 20 : Equilibrium PN Junctions I Class Outline:
ECE 340 Lecture 20 : Equilibrium PN Junctions I Class Outline: Fabrication of pn junctions Contact Potential Things you should know when you leave Key Questions What are the necessary steps to fabricate
More informationModule  01 Lecture  23 The Diffusion Equation
Electronic Materials Devices and Fabrication Layering: Thermal Oxidation Dr. S. Parasuraman Department of Metallurgical and Materials Engineering Indian Institute of Technology, Madras Module  01 Lecture
More informationCHEMICAL BONDING IONIC & METALLIC BONDS
CHEMICAL BONDING IONIC & METALLIC BONDS Mutual electrical attraction between the nuclei and valence electrons of different atoms that binds the atoms together When atoms form chemical bonds they have Lower
More informationv kt = N A ρ Au exp (
42 4.2 Determination of the number of vacancies per cubic meter in gold at 900 C (1173 K) requires the utilization of Equations 4.1 and 4.2 as follows: N v N exp Q v N A ρ Au kt A Au exp Q v kt (6.023
More informationPhase Transformations in Metals and Alloys
Phase Transformations in Metals and Alloys THIRD EDITION DAVID A. PORTER, KENNETH E. EASTERLING, and MOHAMED Y. SHERIF ( г йс) CRC Press ^ ^ ) Taylor & Francis Group Boca Raton London New York CRC Press
More informationMet2023: Concepts of Materials Science I Sample Questions & Answers,(2009) ( Met, PR, FC, MP, CNC, McE )
1 Met223: Concepts of Materials Science I Sample Questions & Answers,(29) ( Met, PR, FC, MP, CNC, McE ) Q1.Define the following. (i) Point Defects (ii) Burgers Vector (iii) Slip and Slip system (iv)
More informationMCEN 2024, Spring 2008 The week of Apr 21 HW 10 Final
MCEN 2024, Spring 2008 The week of Apr 21 HW 10 Final The Quiz questions based upon HW10 will open on Thursday, Apr. 24 and close on Monday, Apr 28 at 1:30 PM. References to A&J: Topic: High Temperature
More informationPhases and Microstructure
Phases and Microstructure 1 FeFe3C phase diagram Iron and Steel Steel Microstructures IronIron carbide phase diagram 0.18 0.10 2.11 0.77 0.008 at RT Identify the terminal phases and its solubility Dr.
More informationMechanisms of Diffusion in Materials 3.205 L4 11/7/06
Mechanisms of Diffusion in Materials 1 A final point on interdiffusion The composition profiles resulting from interdiffusion are generally constrained by phase equilibria. Consider the an Ir Re diffusion
More informationLecture 2 The Vacancy
Lecture 2 The Vacancy Imperfections in Nearly Perfect Crystals There is a book by this title, edited by W. Shockley, J.H. Hollomon, R. Maurer, F. Seitz, published by John Wiley & Sons, in 1952. I found
More informationChapter 2 SolidState Electronics
Chapter 2 SolidState Electronics Microelectronic Circuit Design Richard C. Jaeger Travis N. Blalock Chap 21 Chapter Goals Explore semiconductors and discover how engineers control semiconductor properties
More informationFast Diffusion of Metastable Vacancies in Surface of Excited Si Crystals
Vol. 110 (2006) ACTA PHYSICA POLONICA A No. 4 Fast Diffusion of Metastable Vacancies in Surface of Excited Si Crystals A.J. Janavičius a, and S. Turskienė b a Faculty of Natural Sciences, Šiauliai University
More informationName: Date: Topic: Bonding Classwork. Listening to Some Metal
Name: Date: Topic: Bonding Classwork Learning Objective: Listening to Some Metal 2.20 The student is able to explain how a bonding model involving delocalized electrons is consistent with macroscopic properties
More informationQuestion 6.5: A steel bar 100 mm (4.0 in.) long and having a square cross section 20 mm
14:440:407 Ch6 Question 6.3: A specimen of aluminum having a rectangular cross section 10 mm 12.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationMethods of Heat Transfer
Methods of Heat Transfer Thermodynamics often makes reference to the heat transfer betwen systems. Often these laws do not adequately describe heat transfer processes, so we must introduce more accurate
More informationProcessing of Semiconducting Materials Prof. Pallab Banerji Department of Metallurgy and Material Science Indian Institute of Technology, Kharagpur
Processing of Semiconducting Materials Prof. Pallab Banerji Department of Metallurgy and Material Science Indian Institute of Technology, Kharagpur Lecture  8 Diffusion and Ion Implantation II (Refer
More informationIronCarbon Phase Diagram (a review) see Callister Chapter 9
IronCarbon Phase Diagram (a review) see Callister Chapter 9 University of Tennessee, Dept. of Materials Science and Engineering 1 The Iron Iron Carbide (Fe Fe 3 C) Phase Diagram In their simplest form,
More informationELEMENTARY BAND THEORY
ELEMENTARY BAND THEORY PHYSICIST Solid state band Valence band, VB Conduction band, CB Fermi energy, E F Bloch orbital, delocalized ndoping pdoping Band gap, E g Direct band gap Indirect band gap Phonon
More informationChapter 8. Phase Diagrams
Phase Diagrams A phase in a material is a region that differ in its microstructure and or composition from another region Al Al 2 CuMg H 2 O(solid, ice) in H 2 O (liquid) 2 phases homogeneous in crystal
More informationThe Chemical Bond chemical bond
The Chemical Bond All compounds around us in the universe are formed when atoms combine together. But what holds atoms together once they have combined? Why do some atoms join or bond with others, while
More information